Single-walled carbon nanotube interactions with HeLa cells
© Yehia et al; licensee BioMed Central Ltd. 2007
Received: 10 August 2007
Accepted: 23 October 2007
Published: 23 October 2007
This work concerns exposing cultured human epithelial-like HeLa cells to single-walled carbon nanotubes (SWNTs) dispersed in cell culture media supplemented with serum. First, the as-received CoMoCAT SWNT-containing powder was characterized using scanning electron microscopy and thermal gravimetric analyses. Characterizations of the purified dispersions, termed DM-SWNTs, involved atomic force microscopy, inductively coupled plasma – mass spectrometry, and absorption and Raman spectroscopies. Confocal microRaman spectroscopy was used to demonstrate that DM-SWNTs were taken up by HeLa cells in a time- and temperature-dependent fashion. Transmission electron microscopy revealed SWNT-like material in intracellular vacuoles. The morphologies and growth rates of HeLa cells exposed to DM-SWNTs were statistically similar to control cells over the course of 4 d. Finally, flow cytometry was used to show that the fluorescence from MitoSOX™ Red, a selective indicator of superoxide in mitochondria, was statistically similar in both control cells and cells incubated in DM-SWNTs. The combined results indicate that under our sample preparation protocols and assay conditions, CoMoCAT DM-SWNT dispersions are not inherently cytotoxic to HeLa cells. We conclude with recommendations for improving the accuracy and comparability of carbon nanotube (CNT) cytotoxicity reports.
The structural and electronic properties of SWNTs lend themselves to a variety of biomedical applications involving the detection and treatment of diseases, most notably cancer [1–6]. For example, the structural change in DNA upon shifting from the B to Z conformation sufficiently perturbs the electronic structure of SWNTs such that the change can be detected optically from living cells that have taken up DNA-SWNT complexes . This and other works demonstrate how CNTs can be used as sensors within living cells [8, 9]. In another example, exposing cells containing SWNTs to near infrared radiation kills the cells due to the efficient optical-to-thermal energy conversion of SWNTs, demonstrating that they can potentially be used in targeted cancer therapies to eliminate cancer cells . Finally, there are a number of reports that CNTs facilitate the transport of bound oligonucleotides, peptides, and proteins across the plasma membrane [1, 11–19]. However, despite these and other intracellular applications not listed here, there remain technical challenges towards realizing the potential benefits of CNTs in biomedicine. Namely, CNTs are extremely hydrophobic, bundle together, and are insoluble in water.
Two approaches have been used to modify the hydrophobic surface of CNTs to make them water soluble and biocompatible. The first has been to debundle and disperse CNTs in aqueous solution by covalently attaching water soluble substances to the CNT surface, and the second has involved the noncovalent association of material to the CNT surface [20–26]. In both approaches, a wide variety of organic adducts and biological materials have been used successfully including oligonucleotides [7, 9, 10, 15, 17, 18, 27–40], peptides [14, 19, 41–52], proteins [8, 11–13, 16, 53–59] (most notably, bovine serum albumin (BSA) [60–63]), an assortment of polymers , and various cell culture media formulations [19, 43, 65–72]. While covalently attaching material to CNTs is advantageous for many applications, one serious drawback is that the covalent attachment introduces defects in the surface of the CNTs that often interfere with the electronic and optical properties that make CNTs so useful.
Beyond CNT dispersal, another challenge in the field is assessing whether CNTs are inherently cytotoxic [73–80]. At present, there are roughly as many publications reporting no apparent cytotoxicity [10, 12–14, 16–19, 65–67, 71, 81–87], as there are reporting varying degrees of significant cytotoxicity [68–70, 72, 88–95]. Two major considerations in this area are how the CNTs are presented to the organism and the purity and concentration of the CNTs. For example, pulmonary toxicity of SWNTs has been established when large doses of dry, unpurified SWNTs have been blown into the lungs of rats [89, 90, 96]. This method of presentation is not relevant to the small measured doses of CNTs that would be used in chemotherapy and drug delivery. In fact, the biodistribution of chemically modified SWNTs injected into mice or rabbits was studied recently, and the CNTs were reported to be cleared rapidly with no evidence of toxicity [85, 97, 98]. CNT purity is also absolutely crucial. Many CNT syntheses use metal catalysts that are known to be toxic. Such impurities, and other carbonaceous impurities, must be removed from the samples in order to reach conclusions about inherent CNT toxicity, and it is not always clear from the published reports that they have been removed. Finally, many accounts of CNT toxicity have used MTT (3-(4,5-dimethyl-2-thiazolyl)-2,5-diphenyl-2H-tetrazolium bromide) as a reporter of cell viability, and it was recently shown by Worle-Knirsch et al. that MTT itself binds to CNTs (quenching its fluorescence) and thereby introducing uncertainty in this assessment of toxicity . In summary, while the question of whether CNTs have long-term toxicity in biomedical applications requires further research, early reports raising the alarm of toxicity in model cell culture systems have not been adequately verified.
Recently, our group reported that HiPco SWNTs, dispersed in a peptide solution or in media supplemented with serum, were taken up by HeLa cells in a time- and temperature-dependent fashion and did not affect the HeLa cell growth rate, evidence that the SWNTs inside cells were not toxic under these conditions . This work also demonstrated that our dispersion preparation protocol (involving probe sonication and multiple centrifugations) was effective in removing metals from the raw, as-received SWNT-containing powder. Herein, we present the characterizations of an as-received CoMoCAT SWNT-containing powder using thermal gravimetric analysis (TGA) and scanning electron microscopy (SEM), and of SWNTs dispersed in Dulbecco's modified Eagle medium (DMEM) supplemented with fetal bovine serum (FBS) using atomic force microscopy (AFM), inductively coupled plasma – mass spectrometry (ICP-MS), and absorption and Raman spectroscopies. The resulting purified dispersions, termed DM-SWNTs, are next shown to have no effect upon the morphologies and growth rates of HeLa cells – a thoroughly characterized human epithelial-like cell line. Using confocal microRaman spectroscopy, it is shown that DM-SWNTs were taken up by cells in a time- and temperature-dependent fashion. Evaluation of the distribution of intracellular DM-SWNTs was performed using transmission electron microscopy (TEM) which revealed SWNT-like material in vacuoles. Finally, intracellular superoxide dynamics of cells exposed to DM-SWNTs were evaluated using fluorescence-based flow cytometry and MitoSOX™ Red – a selective indicator of superoxide in mitochondria. The MitoSOX™ Red fluorescence detected from control cells was statistically similar to that observed for cells incubated in DM-SWNT dispersions. The combined results indicate that under our sample preparation protocols and assay conditions, CoMoCAT DM-SWNTs are not inherently cytotoxic to HeLa cells.
Results and Discussion
Characterizations of the as-received SWNT-containing powder
Thermal gravimetric analyses
Characterizations of SWNT dispersions
While a variety of cell types have been cultured in pristine or functionalized CNTs solubilized in various growth media formulations [19, 43, 65–72], only a few of these reports have emphasized the important role that the added serum plays. The importance of FBS in dispersing SWNTs is evident in the series of Raman spectra shown in Figure 4. In brief, DMEM comprises inorganic salts, amino acids, buffers, vitamins, and minerals with the three major components being glucose (4500 mg/L), sodium bicarbonate (3700 mg/L), and sodium chloride (6400 mg/L). FBS is also a multi-component mixture comprising many low and high molecular weight substances. The major dissolved substances are proteins, lipids, steroid hormones, minerals, and metabolites. The most notable FBS components known to solubilize CNTs are BSA and phospholipids [10, 53, 58]. Using our sonication and centrifugation procedure, DMEM without FBS did not support SWNT dispersion as observed by the lack of detectable SWNT Raman resonances (Figure 4; gold spectrum). Conversely, aqueous 5% FBS solutions (without DMEM) were quite effective in dispersing SWNTs (Figure 4; red spectrum).
Previous elemental analyses of peptide-coated SWNT dispersions prepared using our sonication and centrifugation protocol revealed only trace amounts of metal catalysts even though the as-received HiPco SWNT-containing powder contained ~32% metals by weight . Herein, we further characterize this protocol's ability to effectively remove toxic materials by analyzing CoMoCAT DM-SWNT dispersions. CoMoCAT SWNTs are made from a process that uses Co and Mo as catalysts rather than Fe, and thus, exposing CoMoCAT SWNTs to cells avoids the known cellular toxicity that Fe can impact to a CNT preparation [66, 70]. The ICP-MS analyses of DM-SWNT dispersions revealed 6.64 ppm Mo and 1.55 ppm Co, and that the only Fe in our DM-SWNT dispersions was from the 0.10 ppm ferric nitrate in DMEM. For comparative purposes in the absence of EC50 values for dispersed SWNTs, the metal levels observed in the DM-SWNT dispersions were well below the 90 ppm EC50 of mammalian stem cells exposed to 30-nm MoO3 particles (as determined by MTS assays) , and the 19 ppm EC50 of murine fibroblasts exposed to Co (as determined by MTT assays) . Since >99% of the Mo and Co present in the as-received SWNT-containing powder was not detected in the DM-SWNT dispersions (relative to oxidized metal levels from the TGA of the SWNT-containing powder), these data again demonstrate that our sonication and centrifugation protocol is an effective method for removing the heavier metal-containing SWNTs and bundles. Such results are important to note since it has not been made clear in all previous published reports of cells being exposed to CNTs if such metal-removing measures were implemented before the CNT cytotoxicity was assessed.
DM-SWNTs were additionally analyzed for the presence of Ti since it is possible that this metal could be introduced through the use of Ti-coated probe sonicator tips. ICP-MS analyses of DM-SWNT dispersions prepared using a probe tip that had been used for >20 non-continuous hours revealed 0.15 ppm Ti. For comparison, this level is well below the 250 ppm EC50 of rat liver cells exposed to 40-nm TiO2 particles (as determined by MTT assays) . To our knowledge, this is the first report of such an analysis amongst the previous reports of cells exposed to SWNT dispersions prepared using probe tip sonication.
The uptake of DM-SWNTs by living cells
The main analytical approaches for assessing the presence of CNTs in cells and tissue have been optical [1, 14, 65, 67, 72, 83, 88, 90, 93, 113], electron [11, 15, 17, 37, 68–70, 89, 114], and fluorescence [10, 12–14, 16, 18, 43, 64, 82, 84, 86] microscopies. While optical microscopy is ideally suited for live-cell analyses, this label-free technique lacks the specificity to unambiguously identify material observed in cells as CNTs. Electron microscopy offers high spatial resolution imaging of CNTs but is limited to slices of cells that have been fixed; multi-walled CNTs can be unmistakably identified in cells with this technique. In live-cell fluorescence microscopy, the detection of CNTs is indirect (i.e., it is through the detection of a visible fluorescent dye that is (non)covalently attached to the CNT or to molecules coating the CNT). Recently, direct and label-free mapping of CNTs inside living cells has been demonstrated using the intrinsic near-infrared fluorescence [7, 9, 81] or Raman scattering  of CNTs themselves.
Confocal microRaman spectroscopy of HeLa cells
Temporal evaluation of DM-SWNT uptake by HeLa cells
The intracellular distribution of DM-SWNTs
Conclusive evidence of SWNT-like structures in the nucleus was not observed (compare Figures 8A–E to Figures 9A,B,C,F). This is important to note since there is presently no consensus regarding the ability of SWNTs to enter the cellular nucleus or the mechanism for their entry. For example, data that SWNTs have crossed the nuclear membrane has been presented by Bianco and co-workers using TEM and 300–1000-nm long peptide functionalized multi-walled CNTs , and Lu et al. using radioactive labels and ~400-nm long RNA-modified SWNTs . In contrast, Strano and co-workers used confocal Raman imaging to observe DNA-coated SWNTs in the perinuclear zone of 3T3 cells, but not in the nuclear envelope . In summary, amongst reports presenting high-resolution TEM images of cultured cells and tissue exposed to CNTs [11, 15, 17, 37, 68–70, 89, 114], it is apparent that large multi-walled CNTs can be unmistakably identified in cells by visual observation. The situation is more difficult when cells have been exposed to SWNTs. In most cases, the purported SWNT material appears as a single, dense black mass of material and there are few structural features observable on-scale with the expected diameters of individual/bundled SWNTs (± coatings). In fact, when SWNTs have been observed to be densely internalized in cell vacuoles , there are no observable differences between those TEM images and TEM images of cells exposed to fullerenes, which also display vacuoles densely filled with black material . Clearly, the development of complementary analyses capable of identifying SWNT and NTC species in such images is warranted.
Cell growth studies
Intracellular superoxide dynamics of HeLa cells incubated in DM-SWNTs
As recommended by Worle-Knirsch et al., the presentation of CNT cytotoxicity results should include at least two or more independent test systems . Therefore, in conjunction with morphology and growth rate studies, fluorescence-based flow cytometry was utilized to investigate whether the uptake of DM-SWNTs by HeLa cells increased the production of reactive oxygen species (ROS). In these series of experiments, HeLa cells were incubated in DM-SWNT dispersions and incubated with MitoSOX™ Red – a novel fluorescent indicator for the selective measurement of superoxide (O2•-) production in cells [121–123]. MitoSOX™ Red is a non-fluorescent, cell permeable dye that forms a highly fluorescent product upon oxidation. Owing to its lipophilic triphenyl phosphonium cation, MitoSOX™ Red is selectively targeted to mitochondria – the major source of ROS in cells – where it can be oxidized by superoxide before exhibiting red fluorescence upon binding to nucleic acids .
Figures 12C &12D (and Figures S6C&D in Additional File 4) show representative responses of cells loaded with MitoSOX™ Red and incubated either in a DMEM/FBS control (no SWNTs) or in a DM-SWNT dispersion. The means and standard deviations of fluorescence intensities from these two experiments (51.0 ± 24.2 and 47.3 ± 22.1 a.u. for DMEM/FBS controls and DM-SWNT treated cells, respectively) were statistically similar. For comparison, the mean fluorescence intensities from the positive control shown in Figure 12E (and Figure S6E in Additional File 4) was ~7-fold greater (343 ± 101 a.u.). These results are akin to the results of Shvedova and co-workers who observed interesting relationships between the metal content of SWNTs and the iron-induced intracellular production of ROS. In brief, SWNTs containing 26.0 wt% Fe stimulated significant production of hydroxyl radicals by RAW 264.7 macrophages (vs. purified SWNTs containing 0.23 wt % Fe as detected by electron paramagnetic resonance spin-trapping assays), while fluorescence analyses with dihydroethidium incubated macrophages revealed similar superoxide and nitric oxides levels for both cells exposed to the Fe-containing SWNTs or purified SWNTs . Nonetheless, while superoxide is just one of many potential reactive oxygen and nitrogen species, and while Co, Mo, Ti, and Fe are just four types of potential metal impurities, these data suggest that our preparations and concentrations of purified DM-SWNTs do not increase the concentrations of mitochondrial superoxide in HeLa cells under these culture conditions.
Herein, CoMoCAT SWNT-containing powders and DM-SWNT dispersions were characterized using AFM, ICP-MS, SEM, TGA, and absorption and Raman spectroscopies. Confocal micoRaman spectroscopy was utilized to determine that DM-SWNTs entered HeLa cells in a time- and temperature-dependent fashion. TEM revealed SWNT-like material in intracellular vacuoles. Flow cytometry showed that the fluorescence from MitoSOX™ Red, a selective indicator of superoxide in mitochondria, in control cells was statistically similar to that observed for cells incubated in DM-SWNTs. The morphologies and growth rates of HeLa cells exposed to DM-SWNTs were statistically similar to control cells over the course of 4 d. The combined results indicate that, using our sample preparation protocols (i.e., probe tip sonication followed by two centrifugations), and under our assay conditions (i.e., SWNT types, coatings, dimensions, concentrations, impurity types and amounts, and cellular exposure times), CoMoCAT DM-SWNT dispersions are not inherently cytotoxic to HeLa cells. Finally, the importance of thoroughly characterizing CNT materials before offering a CNT cytotoxicity assessment can not be over emphasized. We support the development of (i) standardized CNT sample preparation protocols, reference materials, and characterization methodologies, (ii) standardized methods for assessing whether CNTs are taken up by and/or adsorbed to cells, and (iii) a series of proven cell vitality assay conditions. Such measures are imperative to improve the accuracy and comparability of CNT cytotoxicity reports.
Media and solutions
Dulbecco's modified Eagle medium (DMEM) was purchased from Irvine Scientific and was supplemented with 3700 mg/L sodium bicarbonate, 1% (v/v) penicillin, streptomycin, and amphotericin B (Sigma-Aldrich). Fetal bovine serum (FBS) was obtained from HyClone. Phosphate buffered saline (PBS; 8 mM phosphate, 150 mM NaCl, pH = 7.4) was sterilized by autoclaving at 120°C for 0.5 h. Deionized water (18.3 MΩ-cm) was obtained using a Nanopure Infinity water purification system (Barnstead). All other chemicals were of the highest quality available and were used as received.
All dispersions were prepared with CoMoCAT SWNTs (Product No. SP95-02-dry, Lot No. UT3-A001; SouthWest NanoTechnologies Inc.). The preparation of DM-SWNTs (i.e., SWNTs dispersed in DMEM supplemented with 5% (v/v) FBS (i.e., DMEM/FBS)) used a sonication/centrifugation protocol identical to that previously described by Chin et al. except that the centrifugation times were reduced . Specifically, 1.0 mg of the as-received SWNT-containing powder was dispensed into an Eppendorf tube containing 1.0 mL of DMEM/FBS, vortexed for ~1 min, and probe sonicated for 10 min at 0°C. Probe-sonication was performed using a Branson 250 Sonifier, and the 2 mm diameter probe tip was placed one-third of the distance below the surface of the 1 mL suspension. The resulting black suspension was centrifuged in an Eppendorf 5417C centrifuge for 2 min at 16,000 g (14,000 RPM). The upper 75% of the supernatant was recovered without disturbing the sediment and placed in a clean tube before a second 2 min centrifugation at 16,000 g was performed. The upper 75% of the second supernatant was carefully recovered to afford a DM-SWNT dispersion. The preparation of aqueous dispersions in 0.15% (v/v) sodium dodecyl sulfate (SDS-SWNTs), 0.1% (v/v) TritonX-100 (TrX-SWNTs), or 5% (v/v) FBS (FBS-SWNTs) was identical to that described above except that DMEM/FBS was replaced by the corresponding surfactant or serum.
Scanning electron microscopy
SEM was performed at 10 kV with a Zeiss-LEO Model 1530 variable pressure field effect scanning electron microscope. Samples of the as-received SWNT-containing powder were placed on a SEM mount with carbon black tape and analyzed without a conductive coating.
Thermal gravimetric analysis
TGA was performed with a Perkin Elmer Pyris-1 thermal gravimetric analyzer equipped with a high temperature furnace and sample thermocouple. Samples (n = 3) of the as-received SWNT-containing powder were dried in air for 6 h at 100°C before being transferred into the platinum pan of the analyzer. The samples were heated from room temperature to 1000°C at 5°C/min in >99.9% O2 using a flow rate of 20 mL/min. A baseline was generated for each scan and baseline-subtracted thermograms were converted to weight percents. Thermal oxidation temperatures were identified by the peaks from the derivative of weight percent curve. Triplicate analyses yielded oxidation temperatures with a reproducibility of ± 2°C. The determination of a component's mass was performed by subtracting the weight percent lost between peak onset and end. In the case where two peaks overlapped (Figure 2, peaks 'a' and 'b'), the weight percent lost for the non-overlapping half of each peak was calculated and doubled. Validation of this approach was performed through a Gaussian peak fitting routine to determine the weight percent loss (i.e., the peak area) of each component; the reported masses from the two methods matched within ± 1%. The total mass of oxidized metal was reported as the sum of the mass from MoO3 (peak 'c') and the mass remaining at 1000°C. Triplicate analyses demonstrated mass accuracies of ± 0.2%. The initial weight loss ≤300°C was ~5%. While additional error could be attributed to weight gain by the oxidation of metals, the major source of error in reported weight percentages emanated from the fitting of peaks with components displaying overlapping oxidation temperatures.
The absorption spectra of DM-SWNTs were acquired using a dual-beam Perkin Elmer Lambda 900 UV-VIS-NIR spectrophotometer and were background-corrected using DMEM/FBS. Scans were performed from 400–861 nm with a scan speed of 125.00 nm/min and a 0.44-s integration time and from 861–1350 nm with a scan speed of 125.00 nm/min and a 0.48-s integration time. The instrument was wavelength calibrated on a quarterly basis using Holmium standards.
Elemental analysis was performed using a ThermoElectron X-Series inductively coupled plasma mass spectrometer. Samples (100 μL of DMEM/FBS or DM-SWNTs) were acid digested using a protocol developed in association with PreciLab Inc. (Addison, TX). In brief, a solution of 25 μL of 37% HCl and 25 μL of 69% HNO3 was added to samples which were bath ultrasonicated for 20 min. Next, the samples were diluted with a 2% HNO3 blank to a total volume of 10 mL. All samples and standard solutions were sprayed into flowing argon and passed into the torch which was inductively heated to ~10,000°C. Ti and Co were calibrated using blank, 50-, 100-, and 250-ppt standard solutions, Mo was calibrated using blank, 250-, 1000-, and 5000-ppt standard solutions, and Fe was calibrated using blank, 0.25-, 1.0- and 5.0-ppb standard solutions.
Primary cell culture
Human epithelial-like HeLa cells were obtained from the American Type Culture Collection and were cultured in 100 mm diameter polystyrene tissue culture dishes (Sarstedt) in DMEM/FBS containing 15 mg/L phenol red in an incubator at 37°C with 90% air and 10% CO2. Aseptic conditions were maintained at all times and media was changed every 2 d. Cells were passaged 1:10 every 4 d upon achieving ~80% confluence.
Population doubling time assays
HeLa cells were plated into standard 24-well plates (~1 × 104 cells/well; ~20% coverage) in DMEM/FBS (buffered with 10 mM HEPES; no bicarbonate) and incubated in air at 37°C. After 24 h, the media was removed and replaced by a 400-μL aliquot of freshly prepared DM-SWNTs or fresh media (control). Each group of cells was incubated further in air at 37°C for 1–4 d. On each day, some HeLa cells were washed twice with 400 μL of sterile PBS and harvested with 100 μL of trypsin-EDTA solution (Irvine Scientific) for Coulter cell counting. Population doubling times (PDTs) were determined using the equation PDT = ln (N/N o )/t, where N o represents the initial cell number, N represents the final cell number, and t represents the time interval between N o and N . Each group of cells was analyzed in triplicate; one-way ANOVA statistical analyses were performed at the 95% confidence level, where p < 0.05 was considered significant. Differential image contrast (DIC) images were acquired using a Nikon TE 2000-U inverted microscope and a 60×/1.4 NA APO-Plan oil-immersion objective.
Confocal microRaman spectroscopy
All Raman spectra acquisition and sample preparation methods were similar to those described previously by Chin et al. . Spectra were acquired utilizing a Horiba Jobin Yvon high-resolution LabRam Raman microscope system equipped with a 250-μm entrance slit and a 400-μm pinhole. The 633-nm laser excitation was provided by a Spectra-Physics model 127 helium-neon laser operating at 20 mW. The power density emanating from the 50×/0.5 NA LM-Plan objective was typically 3.4 mW as measured using a Newport model-1815C power meter with an 818 UV series photodetector. Wavenumber calibration was performed using the 520.5 cm-1 line of a silicon wafer; the spectral resolution was ~1 cm-1.
Raman spectra of SWNT dispersions were acquired by placing them into 35 mm polylysine-coated glass bottom "imaging" dishes (MatTek). The acquisition time for a 250-cm-1 spectral region was 10 s with a scan speed of 0.04 cm-1/s; all spectra were plotted as the average of three scans. For live-cell analyses, ~1 × 105 HeLa cells were seeded in imaging dishes with DMEM/FBS and incubated at 37°C in 90% air and 10% CO2. After 24 h, the media was removed and the HeLa cells were rinsed three times with sterile PBS. The cells were incubated further in air at 37°C (or 4°C) in 1 mL of either DMEM/FBS (control) or a freshly prepared DM-SWNT dispersion. Following the designated DM-SWNT incubation period (12–60 h), the cells were copiously rinsed at least three times with sterile PBS. After excess PBS was removed from the dish, 1 mL of fresh media was added and the dish was placed on the microscope stage for analysis at room temperature. Adherent cells were brought into focus by viewing transmitted white-light images obtained through a CCD video camera. The Raman acquisition time for a 250 cm-1 spectral region was 45 s with a scan speed of 0.18 cm-1/s; all spectra were plotted as the average of three scans.
Transmission electron microscopy
Live cells were incubated in a DM-SWNT dispersion (or a DMEM/FBS control) for 60 h as described above. After the final PBS rinsing, the cells were fixed using 2.5% glutaraldehyde in 0.1 M cacodylate buffer and embedded in agarose. Cell pellets were cut into small pieces, post-fixed with 1% osmium tetroxide, en-bloc stained with 1% uranyl acetate, dehydrated in a graded ethanol series, and embedded in EMbed-812 resin. Ultrathin (~100 nm) sections were cut on a LEICA EM UC6 ultramicrotome, post-stained with uranyl acetate and lead citrate, and viewed using the JEOL JEM-1200EX II electron microscope at the Molecular and Cellular Imaging Facility at The University of Texas Southwestern Medical Center.
In all flow cytometry experiments, ~1.0 × 106 HeLa cells were seeded in imaging dishes with DMEM/FBS and incubated at 37°C in 90% air and 10% CO2. After 24 h, the media was removed, the cells were rinsed with sterile PBS, and the cells were incubated in fresh DMEM/FBS (control) or a DM-SWNT dispersion in air at 37°C for 60 h. In some cases, cells were rinsed at least three times with sterile PBS and loaded with a solution of MitoSOX™ Red (Invitrogen-Molecular Probes). Specifically, cells were incubated for 60 min at 37°C in a 10 μM MitoSOX™ Red solution prepared in 4:1 (v/v) DMEM/PBS. Next, cells were rinsed three times with PBS, harvested with 500 μL of trypsin-EDTA solution, centrifuged at 5000 RPM for 5 min, and resuspended in 3 mL of fresh 2% (v/v) FBS/PBS. Finally, cell suspensions were filtered through a 30-μm PreSeparation filter (Miltenyi Biotec). Fluorescence-based flow cytometry was performed using a Becton Dickinson FACSCalibur ® flow cytometer equipped with a 488 nm laser. MitoSOX™ Red fluorescence (λMax = 590 nm) was detected over the range of 564–606 nm and the background fluorescence was detected over the range of 515–545 nm. All quantitations were performed using CellQuest 7.5.3 software; in each experiment, well over 10,000 cells were analyzed.
This work was supported by grants from the Robert A. Welch Foundation (PP; grant AT-1364 and IHM; grant AT-1326) and the Human Frontier Science Program (GRD; grant RGY0070/2005-C), by the gift of equipment from the von Ehr Foundation, and by funds from the State of Texas (RKD). We are grateful for assistance to this work by Chris Gilpin, Karis Hughes, Laurie Mueller, and Vicky Poenitzsch, and for insightful discussions with Ray Baughman, Alan Dalton, Radu Marches, and Ru-Hung Wang.
- Klumpp C, Kostarelos K, Prato M, Bianco A: Functionalized carbon nanotubes as emerging nanovectors for the delivery of therapeutics. Biochimica et Biophysica Acta, Biomembranes. 2006, 1758: 404-412. 10.1016/j.bbamem.2005.10.008.
- Ferrari M: Nanovector therapeutics. Current Opinion in Chemical Biology. 2005, 9: 343-346. 10.1016/j.cbpa.2005.06.001.
- Ferrari M: Cancer nanotechnology: opportunities and challenges. Nature Reviews Cancer. 2005, 5: 161-171. 10.1038/nrc1566.
- Penn SG, He L, Natan MJ: Nanoparticles for bioanalysis. Current Opinion in Chemical Biology. 2003, 7: 609-615. 10.1016/j.cbpa.2003.08.013.
- Portney NG, Ozkan M: Nano-oncology: drug delivery, imaging, and sensing. Analytical and Bioanalytical Chemistry. 2006, 384: 620-630. 10.1007/s00216-005-0247-7.
- Martin CR, Kohli P: The emerging field of nanotube biotechnology. Nature Reviews Drug Discovery. 2003, 2: 29-37. 10.1038/nrd988.
- Heller DA, Jeng ES, Yeung TK, Martinez BM, Moll AE, Gastala JB, Strano MS: Optical Detection of DNA Conformational Polymorphism on Single-Walled Carbon Nanotubes. Science (Washington, DC, United States). 2006, 311: 508-511. 10.1126/science.1120792.
- Barone PW, Baik S, Heller DA, Strano MS: Near-infrared optical sensors based on single-walled carbon nanotubes. Nature Materials. 2005, 4: 86-92. 10.1038/nmat1276.
- Heller DA, Baik S, Eurell TE, Strano MS: Single-walled carbon nanotube spectroscopy in live cells: Towards long-term labels and optical sensors. Advanced Materials (Weinheim, Germany). 2005, 17: 2793-2799. 10.1002/adma.200500477.
- Kam NWS, O'Connell M, Wisdom JA, Dai H: Carbon Nanotubes as multifunctional biological transporters and near-infrared agents for selective cancer cell destruction. Proceedings of the National Academies of Science. 2005, 102: 11600-11605. 10.1073/pnas.0502680102.
- Lin Y, Zhou B, Martin RB, Henbest KB, Harruff BA, Riggs JE, Guo ZX, Allard LF, Sun YP: Visible Luminescence of Carbon Nanotubes and Dependence on Functionalization. Journal of Physical Chemistry B. 2005, 109: 14779-14782. 10.1021/jp053073j.
- Kam NWS, Dai H: Carbon Nanotubes as Intracellular Protein Transporters: Generality and Biological Functionality. Journal of the American Chemical Society. 2005, 127: 6021-6026. 10.1021/ja050062v.
- Kam NWS, Jessop TC, Wender PA, Dai H: Nanotube molecular transporters: internalization of carbon nanotube-protein conjugates into mammalian cells. Journal of the American Chemical Society. 2004, 126: 6850-6851. 10.1021/ja0486059.
- Pantarotto D, Briand JP, Prato M, Bianco A: Translocation of bioactive peptides across cell membranes by carbon nanotubes. Chemical Communications (Cambridge, United Kingdom). 2004, 16-17. 10.1039/b311254c.
- Pantarotto D, Singh R, McCarthy D, Erhardt M, Briand JP, Prato M, Kostarelos K, Bianco A: Functionalized carbon nanotubes for plasmid DNA gene delivery. Angewandte Chemie, International Edition. 2004, 43: 5242-5246. 10.1002/anie.200460437.
- Wu W, Wieckowski S, Pastorin G, Benincasa M, Klumpp C, Briand JP, Gennaro R, Prato M, Bianco A: Targeted delivery of amphotericin B to cells by using functionalized carbon nanotubes. Angewandte Chemie, International Edition. 2005, 44: 6358-6362. 10.1002/anie.200501613.
- Cai D, Mataraza JM, Qin ZH, Huang Z, Huang J, Chiles TC, Carnahan D, Kempa K, Ren Z: Highly efficient molecular delivery into mammalian cells using carbon nanotube spearing. Nature Methods. 2005, 2: 449-454. 10.1038/nmeth761.
- Lu Q, Moore JM, Huang G, Mount AS, Rao AM, Larcom LL, Ke PC: RNA polymer translocation with single-walled carbon nanotubes. Nano Letters. 2004, 4: 2473-2477. 10.1021/nl048326j.
- Chin SF, Baughman Ray H, Dalton Alan B, Dieckmann Gregg R, Draper Rockford K, Mikoryak C, Musselman Inga H, Poenitzsch VZ, Xie H, Pantano P: Amphiphilic helical peptide enhances the uptake of single-walled carbon nanotubes by living cells. Exp Biol Med (Maywood). 2007, 232 (9): 1236-1244.
- Tasis D, Tagmatarchis N, Bianco A, Prato M: Chemistry of carbon nanotubes. Chemical Reviews. 2006, 106: 1105-1136. 10.1021/cr050569o.
- Lin Y, Taylor S, Li H, Fernando KAS, Qu L, Wang W, Gu L, Zhou B, Sun YP: Advances toward bioapplications of carbon nanotubes. Journal of Materials Chemistry. 2004, 14: 527-541. 10.1039/b314481j.
- Bahr JL, Tour JM: Covalent chemistry of single-wall carbon nanotubes. Journal of Materials Chemistry. 2002, 12: 1952-1958. 10.1039/b201013p.
- Banerjee S, Hemraj-Benny T, Wong SS: Covalent surface chemistry of single-walled carbon nanotubes. Advanced Materials (Weinheim, Germany). 2005, 17: 17-29. 10.1002/adma.200401340.
- Tasis D, Tagmatarchis N, Georgakilas V, Prato M: Soluble carbon nanotubes. Chem Eur J. 2003, 9: 4000-4008. 10.1002/chem.200304800.
- Sun YP, Fu K, Lin Y, Huang W: Functionalized carbon nanotubes: properties and applications. Accounts of Chemical Research. 2002, 35: 1096-1104. 10.1021/ar010160v.
- Niyogi S, Hamon MA, Hu H, Zhao B, Bhowmik P, Sen R, Itkis ME, Haddon RC: Chemistry of Single-Walled Carbon Nanotubes. Accounts of Chemical Research. 2002, 35: 1105-1113. 10.1021/ar010155r.
- Chou SG, Plentz F, Jiang J, Saito R, Nezich D, Ribeiro HB, Jorio A, Pimenta MA, Samsonidze GG, Santos AP, Zheng M, Onoa GB, Semke ED, Dresselhaus G, Dresselhaus MS: Phonon-Assisted Excitonic Recombination Channels Observed in DNA-Wrapped Carbon Nanotubes Using Photoluminescence Spectroscopy. Physical Review Letters. 2005, 94: 127402/1-127402/4. 10.1103/PhysRevLett.94.127402.
- Singh R, Pantarotto D, McCarthy D, Chaloin O, Hoebeke J, Partidos CD, Briand JP, Prato M, Bianco A, Kostarelos K: Binding and Condensation of Plasmid DNA onto Functionalized Carbon Nanotubes: Toward the Construction of Nanotube-Based Gene Delivery Vectors. Journal of the American Chemical Society. 2005, 127: 4388-4396. 10.1021/ja0441561.
- Badaire S, Zakri C, Maugey M, Derre A, Barisci JN, Wallace G, Poulin P: Liquid crystals of DNA-stabilized carbon nanotubes. Advanced Materials (Weinheim, Germany). 2005, 17: 1673-1676. 10.1002/adma.200401741.
- Lustig SR, Jagota A, Khripin C, Zheng M: Theory of structure-based carbon nanotube separations by ion-exchange chromatography of DNA/CNT hybrids. Journal of Physical Chemistry B. 2005, 109: 2559-2566. 10.1021/jp0452913.
- Strano MS, Zheng M, Jagota A, Onoa GB, Heller DA, Barone PW, Usrey ML: Understanding the nature of the DNA-assisted separation of single-walled carbon nanotubes using fluorescence and Raman spectroscopy. Nano Letters. 2004, 4: 543-550. 10.1021/nl034937k.
- Zheng M, Jagota A, Strano MS, Santos AP, Barone P, Chou SG, Diner BA, Dresselhaus MS, McLean RS, Onoa GB, Samsonidze GG, Semke ED, Usrey M, Walls DJ: Structure-Based Carbon Nanotube Sorting by Sequence-Dependent DNA Assembly. Science (Washington, DC, United States). 2003, 302: 1545-1548. 10.1126/science.1091911.
- Zheng M, Jagota A, Semke ED, Diner BA, McLean RS, Lustig SR, Richardson RE, Tassi NG: DNA-assisted dispersion and separation of carbon nanotubes. Nature Materials. 2003, 2: 338-342. 10.1038/nmat877.
- He P, Bayachou M: Layer-by-Layer Fabrication and Characterization of DNA-Wrapped Single-Walled Carbon Nanotube Particles. Langmuir. 2005, 21: 6086-6092. 10.1021/la050581b.
- Li S, He P, Dong J, Guo Z, Dai L: DNA-Directed Self-Assembling of Carbon Nanotubes. Journal of the American Chemical Society. 2005, 127: 14-15. 10.1021/ja0446045.
- Tan S, Lopez HA, Cai CW, Zhang Y: Optical Trapping of Single-Walled Carbon Nanotubes. Nano Letters. 2004, 4: 1415-1419. 10.1021/nl049347g.
- Bianco A, Kostarelos K, Prato M: Applications of carbon nanotubes in drug delivery. Current Opinion in Chemical Biology. 2005, 9: 674-679. 10.1016/j.cbpa.2005.10.005.
- Kam NWS, Liu Z, Dai H: Functionalization of Carbon Nanotubes via Cleavable Disulfide Bonds for Efficient Intracellular Delivery of siRNA and Potent Gene Silencing. Journal of the American Chemical Society. 2005, 127: 12492-12493. 10.1021/ja053962k.
- Rao R, Lee J, Lu Q, Keskar G, Freedman KO, Floyd WC, Rao AM, Ke PC: Single-molecule fluorescence microscopy and Raman spectroscopy studies of RNA bound carbon nanotubes. Applied Physics Letters. 2004, 85: 4228-4230. 10.1063/1.1813631.
- Arnold MS, Stupp SI, Hersam MC: Enrichment of single-walled carbon nanotubes by diameter in density gradients. Nano Letters. 2005, 5: 713-718. 10.1021/nl050133o.
- Arnold MS, Guler MO, Hersam MC, Stupp SI: Encapsulation of Carbon Nanotubes by Self-Assembling Peptide Amphiphiles. Langmuir. 2005, 21: 4705-4709. 10.1021/la0469452.
- Pantarotto D, Partidos CD, Graff R, Hoebeke J, Briand JP, Prato M, Bianco A: Synthesis, Structural Characterization, and Immunological Properties of Carbon Nanotubes Functionalized with Peptides. J Am Chem Soc. 2003, 125: 6160-6164. 10.1021/ja034342r.
- Bianco A, Kostarelos K, Partidos CD, Prato M: Biomedical applications of functionalized carbon nanotubes. Chemical Communications (Cambridge, United Kingdom). 2005, 571-577. 10.1039/b410943k.
- Wang S, Humphreys ES, Chung SY, Delduco DF, Lustig SR, Wang H, Parker KN, Rizzo NW, Subramoney S, Chiang YM, Jagota A: Peptides with selective affinity for carbon nanotubes. Nature Materials. 2003, 2: 196-200. 10.1038/nmat833.
- Dieckmann GR, Dalton AB, Johnson PA, Razal J, Chen J, Giordano GM, Munoz E, Musselman IH, Baughman RH, Draper RK: Controlled Assembly of Carbon Nanotubes by Designed Amphiphilic Peptide Helices. Journal of the American Chemical Society. 2003, 125: 1770-1777. 10.1021/ja029084x.
- Zorbas V, Ortiz-Acevedo A, Dalton AB, Yoshida MM, Dieckmann GR, Draper RK, Baughman RH, Jose-Yacaman M, Musselman IH: Preparation and Characterization of Individual Peptide-Wrapped Single-Walled Carbon Nanotubes. Journal of the American Chemical Society. 2004, 126: 7222-7227. 10.1021/ja049202b.
- Dalton AB, Ortiz-Acevedo A, Zorbas V, Brunner E, Sampson WM, Collins S, Razal JM, Yoshida MM, Baughman RH, Draper RK, Musselman IH, Jose-Yacaman M, Dieckmann GR: Hierarchical self-assembly of peptide-coated carbon nanotubes. Advanced Functional Materials. 2004, 14: 1147-1151. 10.1002/adfm.200400190.
- Ortiz-Acevedo A, Dieckmann GR: Synthesis of reversible cyclic peptides. Tetrahedron Letters. 2004, 45: 6795-6798. 10.1016/j.tetlet.2004.07.041.
- Xie H, Ortiz-Acevedo A, Zorbas V, Baughman RH, Draper RK, Musselman IH, Dalton AB, Dieckmann GR: Peptide cross-linking modulated stability and assembly of peptide-wrapped single-walled carbon nanotubes. Journal of Materials Chemistry. 2005, 15: 1734-1741. 10.1039/b413262a.
- Zorbas V, Smith AL, Xie H, Ortiz-Acevedo A, Dalton AB, Dieckmann GR, Draper RK, Baughman RH, Musselman IH: Importance of aromatic content for peptide/single-walled carbon nanotube interactions. J Am Chem Soc. 2005, 127: 12323-12328. 10.1021/ja050747v.
- Ortiz-Acevedo A, Xie H, Zorbas V, Sampson WM, Dalton AB, Baughman RH, Draper RK, Musselman IH, Dieckmann GR: Diameter-Selective Solubilization of Single-Walled Carbon Nanotubes by Reversible Cyclic Peptides. Journal of the American Chemical Society. 2005, 127: 9512-9517. 10.1021/ja050507f.
- In het Panhuis M, Gowrisanker S, Vanesko DJ, Mire CA, Jia H, Xie H, Baughman RH, Musselman IH, Gnade BE, Dieckmann GR, Draper RK: Nanotube network transistors from peptide-wrapped single-walled carbon nanotubes. Small. 2005, 1: 820-823. 10.1002/smll.200500001.
- Karajanagi SS, Yang H, Asuri P, Sellitto E, Dordick JS, Kane RS: Protein-Assisted Solubilization of Single-Walled Carbon Nanotubes. Langmuir. 2006, 22: 1392-1395. 10.1021/la0528201.
- Chen RJ, Bangsaruntip S, Drouvalakis KA, Kam NWS, Shim M, Li Y, Kim W, Utz PJ, Dai H: Noncovalent functionalization of carbon nanotubes for highly specific electronic biosensors. Proceedings of the National Academy of Sciences of the United States of America. 2003, 100: 4984-4989. 10.1073/pnas.0837064100.
- Balavoine F, Schultz P, Richard C, Mallouh V, Ebbesen TW, Mioskowski C: Helical crystallization of proteins on carbon nanotubes: a first step towards the development of new biosensors. Angewandte Chemie, International Edition. 1999, 38: 1912-1915. 10.1002/(SICI)1521-3773(19990712)38:13/14<1912::AID-ANIE1912>3.0.CO;2-2.
- Chen RJ, Zhang Y, Wang D, Dai H: Noncovalent sidewall functionalization of single-walled carbon nanotubes for protein immobilization. Journal of the American Chemical Society. 2001, 123: 3838-3839. 10.1021/ja010172b.
- Azamian Bobak R, Davis Jason J, Coleman Karl S, Bagshaw Claire B, Green Malcolm LH: Bioelectrochemical single-walled carbon nanotubes. Journal of the American Chemical Society. 2002, 124: 12664-12665. 10.1021/ja0272989.
- Lin Y, Allard LF, Sun YP: Protein-Affinity of Single-Walled Carbon Nanotubes in Water. Journal of Physical Chemistry B. 2004, 108: 3760-3764. 10.1021/jp031248o.
- Shim M, Kam NWS, Chen RJ, Li Y, Dai H: Functionalization of carbon nanotubes for biocompatibility and biomolecular recognition. Nano Letters. 2002, 2: 285-288. 10.1021/nl015692j.
- Elkin T, Jiang X, Taylor S, Lin Y, Gu L, Yang H, Brown J, Collins S, Sun YP: Immuno-carbon nanotubes and recognition of pathogens. ChemBioChem. 2005, 6: 640-643. 10.1002/cbic.200400337.
- Fu K, Huang W, Lin Y, Zhang D, Hanks TW, Rao AM, Sun YP: Functionalization of carbon nanotubes with bovine serum albumin in homogeneous aqueous solution. Journal of Nanoscience and Nanotechnology. 2002, 2: 457-461. 10.1166/jnn.2002.135.
- Huang W, Taylor S, Fu K, Lin Y, Zhang D, Hanks TW, Rao AM, Sun YP: Attaching proteins to carbon nanotubes via diimide-activated amidation. Nano Letters. 2002, 2: 311-314. 10.1021/nl010095i.
- Lu Q, Freedman KO, Rao R, Huang G, Lee J, Larcom LL, Rao AM, Ke PC: Diffusion of carbon nanotubes with single-molecule fluorescence microscopy. Journal of Applied Physics. 2004, 96: 6772-6775. 10.1063/1.1815053.
- Jiang K, Schadler LS, Siegel RW, Zhang X, Zhang H, Terrones M: Protein immobilization on carbon nanotubes via a two-step process of diimide-activated amidation. Journal of Materials Chemistry. 2004, 14: 37-39. 10.1039/b310359e.
- Worle-Knirsch JM, Pulskamp K, Krug HF: Oops they did it again! Carbon nanotubes hoax scientists in viability assays. Nano letters. 2006, 6: 1261-1268. 10.1021/nl060177c.
- Kagan VE, Tyurina YY, Tyurin VA, Konduru NV, Potapovich AI, Osipov AN, Kisin ER, Schwegler-Berry D, Mercer R, Castranova V, Shvedova AA: Direct and indirect effects of single walled carbon nanotubes on RAW 264.7 macrophages: Role of iron. Toxicology Letters. 2006, 165: 88-100. 10.1016/j.toxlet.2006.02.001.
- Garibaldi S, Brunelli C, Bavastrello V, Ghigliotto G, Nicolini C: Carbon nanotube biocompatibility with cardiac muscle cells. Nanotechnology. 2006, 17: 391-397. 10.1088/0957-4484/17/2/008.
- Monteiro-Riviere NA, Nemanich RJ, Inman AO, Wang YY, Riviere JE: Multi-walled carbon nanotube interactions with human epidermal keratinocytes. Toxicology Letters. 2005, 155: 377-384. 10.1016/j.toxlet.2004.11.004.
- Jia G, Wang H, Yan L, Wang X, Pei R, Yan T, Zhao Y, Guo X: Cytotoxicity of Carbon Nanomaterials: Single-Wall Nanotube, Multi-Wall Nanotube, and Fullerene. Environmental Science and Technology. 2005, 39: 1378-1383. 10.1021/es048729l.
- Shvedova A, Castranova V, Kisin E, Schwegler-Berry D, Murray A, Gandelsman V, Maynard A, Baron P: Exposure to Carbon Nanotube Material: Assessment of Nanotube Cytotoxicity using Human Keratinocyte Cells. J Toxicology and Environmental Health, Part A. 2003, 66: 1909-1926. 10.1080/713853956.
- Flahaut E, Durrieu MC, Remy-Zolghadri M, Bareille R, Baquey C: Investigation of the cytotoxicity of CCVD carbon nanotubes towards human umbilical vein endothelial cells. Carbon. 2006, 44: 1093-1099. 10.1016/j.carbon.2005.11.007.
- Magrez A, Kasas S, Salicio V, Pasquier N, Seo JW, Celio M, Catsicas S, Schwaller B, Forro L: Cellular Toxicity of Carbon-Based Nanomaterials. Nano Letters. 2006, 6: 1121-1125. 10.1021/nl060162e.
- Oberdorster G, Maynard A, Donaldson K, Castranova V, Fitzpatrick J, Ausman K, Carter J, Karn B, Kreyling W, Lai D, Olin S, Monteiro-Riviere N, Warheit D, Yang H: Principles for characterizing the potential human health effects from exposure to nanomaterials: Elements of a screening strategy. Particle and Fibre Toxicology. 2005, 2: 8-43. 10.1186/1743-8977-2-8.
- Nel A, Xia T, Madler L, Li N: Toxic potential of materials at the nanolevel. Science. 2006, 311: 622-627. 10.1126/science.1114397.
- Lam CW, James JT, McCluskey R, Arepalli S, Hunter RL: A Review of Carbon Nanotube Toxicity and Assessment of Potential Occupational and Environmental Health Risks. Critical Reviews in Toxicology. 2006, 36: 189-217. 10.1080/10408440600570233.
- Monteiro-Riviere NA, Inman AO: Challenges for assessing carbon nanomaterial toxicity to the skin. Carbon. 2006, 44: 1070-1078. 10.1016/j.carbon.2005.11.004.
- Panessa-Warren BJ, Warren JB, Wong SS, Misewich JA: Biological cellular response to carbon nanoparticle toxicity. Journal of Physics: Condensed Matter. 2006, 18: S2185-S2201. 10.1088/0953-8984/18/33/S34.
- Smart SK, Cassady AI, Lu GQ, Martin DJ: The biocompatibility of carbon nanotubes. Carbon. 2006, 44: 1034-1047. 10.1016/j.carbon.2005.10.011.
- Oberdorster G, Oberdorster E, Oberdorster J: Nanotoxicology: an emerging discipline evolving from studies of ultrafine particles. Environmental Health Perspectives. 2005, 113: 823-839.
- Kagan VE, Bayir H, Shvedova AA: Nanomedicine and nanotoxicology: Two sides of the same coin. Nanomedicine. 2005, 1: 313-316.
- Cherukuri P, Bachilo SM, Litovsky SH, Weisman RB: Near-infrared fluorescence microscopy of single-walled carbon nanotubes in phagocytic cells. Journal of the American Chemical Society. 2004, 126: 15638-15639. 10.1021/ja0466311.
- Chen X, Tam UC, Czlapinski JL, Lee GS, Rabuka D, Zettl A, Bertozzi CR: Interfacing Carbon Nanotubes with Living Cells. Journal of the American Chemical Society. 2006, 128: 6292-6293. 10.1021/ja060276s.
- Koyama S, Endo M, Kim YA, Hayashi T, Yanagisawa T, Osaka K, Koyama H, Haniu H, Kuroiwa N: Role of systemic T-cells and histopathological aspects after subcutaneous implantation of various carbon nanotubes in mice. Carbon. 2006, 44: 1079-1092. 10.1016/j.carbon.2005.08.006.
- Zhu Y, Ran T, Li Y, Guo J, Li W: Dependence of the cytotoxicity of MWCNTs on the culture medium. Nanotechnology. 2006, 17: 4668-4674. 10.1088/0957-4484/17/18/024.
- Singh R, Pantarotto D, Lacerda L, Pastorin G, Klumpp C, Prato M, Bianco A, Kostarelos K: Tissue biodistribution and blood clearance rates of intravenously administered carbon nanotube radiotracers. Proceedings of the National Academy of Sciences of the United States of America. 2006, 103: 3357-3362. 10.1073/pnas.0509009103.
- Dumortier H, Lacotte S, Pastorin G, Marega R, Wu W, Bonifazi D, Briand JP, Prato M, Muller S, Bianco A: Functionalized carbon nanotubes are non-cytotoxic and preserve the functionality of primary immune cells. Nano Lett. 2006, 6: 1522-1528. 10.1021/nl061160x.
- Hu H, Ni Y, Montana V, Haddon RC, Parpura V: Chemically functionalized carbon nanotubes as substrates for neuronal growth. Nano Letters. 2004, 4: 507-511. 10.1021/nl035193d.
- Cui D, Tian F, Ozkan CS, Wang M, Gao H: Effect of single wall carbon nanotubes on human HEK293 cells. Toxicology Letters. 2005, 155: 73-85. 10.1016/j.toxlet.2004.08.015.
- Lam CW, James JT, McCluskey R, Hunter RL: Pulmonary Toxicity of Single-Wall Carbon Nanotubes in Mice 7 and 90 Days After Intratracheal Instillation. Toxicolology Sciences. 2004, 77: 126-134. 10.1093/toxsci/kfg243.
- Warheit DB, Laurence BR, Reed KL, Roach DH, Reynolds GAM, Webb TR: Comparative Pulmonary Toxicity Assessment of Single-wall Carbon Nanotubes in Rats. Toxicological Sciences. 2004, 77: 117-125. 10.1093/toxsci/kfg228.
- Manna SK, Sarkar S, Barr J, Wise K, Barrera EV, Jejelowo O, Rice-Ficht AC, Ramesh GT: Single-Walled Carbon Nanotube Induces Oxidative Stress and Activates Nuclear Transcription Factor-kB in Human Keratinocytes. Nano Letters. 2005, 5: 1676-1684. 10.1021/nl0507966.
- Ding L, Stilwell J, Zhang T, Elboudwarej O, Jiang H, Selegue JP, Cooke PA, Gray JW, Chen FF: Molecular Characterization of the Cytotoxic Mechanism of Multiwall Carbon Nanotubes and Nano-Onions on Human Skin Fibroblast. Nano Letters. 2005, 5: 2448-2464. 10.1021/nl051748o.
- Sayes CM, Liang F, Hudson JL, Mendez J, Guo W, Beach JM, Moore VC, Doyle CD, West JL, Billups WE, Ausman KD, Colvin VL: Functionalization density dependence of single-walled carbon nanotubes cytotoxicity in vitro. Toxicology Letters. 2006, 161: 135-142. 10.1016/j.toxlet.2005.08.011.
- Chlopek J, Czajkowska B, Szaraniec B, Frackowiak E, Szostak K, Beguin F: In vitro studies of carbon nanotubes biocompatibility. Carbon. 2006, 44: 1106-1111. 10.1016/j.carbon.2005.11.022.
- Templeton RC, Ferguson PL, Washburn KM, Scrivens WA, Chandler GT: Life-cycle effects of single-walled carbon nanotubes (SWNTs) on an estuarine meiobenthic copepod. Environ Sci Technol. 2006, 40 (23): 7387-7393. 10.1021/es060407p.
- Warheit DB: What is currently known about the health risks related to carbon nanotube exposures?. Carbon. 2006, 44: 1064-1069. 10.1016/j.carbon.2005.10.013.
- Cherukuri P, Gannon CJ, Leeuw TK, Schmidt HK, Smalley RE, Curley SA, Weisman RB: Mammalian pharmacokinetics of carbon nanotubes using intrinsic near-infrared fluorescence. Proc Natl Acad Sci U S A. 2006, 103: 18882-18886. 10.1073/pnas.0609265103.
- Liu Z, Cai W, He L, Nakayama N, Chen K, Sun X, Chen X, Dai H: In vivo biodistribution and highly efficient tumour targeting of carbon nanotubes in mice. Nat Nano. 2007, 2: 47-52. 10.1038/nnano.2006.170.
- Herrera JE, Balzano L, Borgna A, Alvarez WE, Resasco DE: Relationship between the structure/composition of Co-Mo catalysts and their ability to produce single-walled carbon nanotubes by CO disproportionation. Journal of Catalysis. 2001, 204: 129-145. 10.1006/jcat.2001.3383.
- Alvarez WE, Pompeo F, Herrera JE, Balzano L, Resasco DE: Characterization of Single-Walled Carbon Nanotubes (SWNTs) Produced by CO Disproportionation on Co-Mo Catalysts. Chemistry of Materials. 2002, 14: 1853-1858. 10.1021/cm011613t.
- Herrera JE, Balzano L, Pompeo F, Resasco DE: Raman characterization of single-walled nanotubes of various diameters obtained by catalytic disproportionation of CO. Journal of Nanoscience and Nanotechnology. 2003, 3: 133-138. 10.1166/jnn.2003.153.
- Bachilo SM, Balzano L, Herrera JE, Pompeo F, Resasco DE, Weisman RB: Narrow (n,m)-Distribution of Single-Walled Carbon Nanotubes Grown Using a Solid Supported Catalyst. Journal of the American Chemical Society. 2003, 125: 11186-11187. 10.1021/ja036622c.
- Lolli G, Zhang L, Balzano L, Sakulchaicharoen N, Tan Y, Resasco DE: Tailoring (n,m) Structure of Single-Walled Carbon Nanotubes by Modifying Reaction Conditions and the Nature of the Support of CoMo Catalysts. Journal of Physical Chemistry B. 2006, 110: 2108-2115. 10.1021/jp056095e.
- SouthWest NanoTechnologies: www.swnano.com/technology. [http://swentnano.com/index.php?page=what-are-swnt-nanotubes]
- Buffa F, Hu H, Resasco DE: Side-Wall Functionalization of Single-Walled Carbon Nanotubes with 4-Hydroxymethylaniline Followed by Polymerization of e-Caprolactone. Macromolecules. 2005, 38: 8258-8263. 10.1021/ma050876w.
- Attal S, Thiruvengadathan R, Regev O: Determination of the concentration of single-walled carbon nanotubes in aqueous dispersions using UV-visible absorption spectroscopy. Anal Chem. 2006, 78: 8098-8104. 10.1021/ac060990s.
- Dresselhaus MS, Dresselhaus G, Jorio A, Souza Filho AG, Saito R: Raman spectroscopy on isolated single wall carbon nanotubes. Carbon. 2002, 40: 2043-2061. 10.1016/S0008-6223(02)00066-0.
- Resasco DE, Herrera JE: Structural characterization of single-walled carbon nanotubes. Encyclopedia of Nanoscience and Nanotechnology. 2004, 10: 125-147.
- Itkis ME, Perea DE, Jung R, Niyogi S, Haddon RC: Comparison of Analytical Techniques for Purity Evaluation of Single-Walled Carbon Nanotubes. Journal of the American Chemical Society. 2005, 127: 3439-3448. 10.1021/ja043061w.
- Braydich-Stolle L, Hussain S, Schlager JJ, Hofmann MC: In vitro cytotoxicity of nanoparticles in mammalian germline stem cells. Toxicological Sciences. 2005, 88: 412-419. 10.1093/toxsci/kfi256.
- Sauvant MP, Pepin D, Bohatier J, Groliere CA, Guillot J: Toxicity assessment of 16 inorganic environmental pollutants by six bioassays. Ecotoxicology and Environmental Safety. 1997, 37: 131-140. 10.1006/eesa.1997.1519.
- Hussain SM, Hess KL, Gearhart JM, Geiss KT, Schlager JJ: In vitro toxicity of nanoparticles in BRL 3A rat liver cells. Toxicology in Vitro. 2005, 19: 975-983. 10.1016/j.tiv.2005.06.034.
- Bianco A: Carbon nanotubes for the delivery of therapeutic molecules. Expert Opinion on Drug Delivery. 2004, 1: 57-65. 10.1517/17425247.1.1.57.
- Kostarelos K, Lacerda L, Partidos CD, Prato M, Bianco A: Carbon nanotube-mediated delivery of peptides and genes to cells: Translating nanobiotechnology to therapeutics. Journal of Drug Delivery Science and Technology. 2005, 15: 41-47.
- Huang YS, Karashima T, Yamamoto M, Ogura T, Hamaguchi H: Raman spectroscopic signature of life in a living yeast cell. Journal of Raman Spectroscopy. 2004, 35: 525-526. 10.1002/jrs.1219.
- Krafft C, Knetschke T, Funk RHW, Salzer R: Studies on Stress-Induced Changes at the Subcellular Level by Raman Microspectroscopic Mapping. Analytical Chemistry. 2006, 78: 4424-4429. 10.1021/ac060205b.
- Cheng JX, Xie XS: Coherent Anti-Stokes Raman Scattering Microscopy: Instrumentation, Theory, and Applications. Journal of Physical Chemistry B. 2004, 108: 827-840. 10.1021/jp035693v.
- Chin SF: Synthetic nano-1 peptide increases the uptake of single-walled carbon nanotubes by HeLa cells. Chemistry. Richardson, Ph.D. Thesis, The University of Texas at Dallas, 2005.
- Yamawaki H, Iwai N: Cytotoxicity of water-soluble fullerene in vascular endothelial cells. American Journal of Physiology. 2006, 290: C1495-C1502. 10.1152/ajpcell.00481.2005.
- Martin BM: Tissue Culture Techniques. Boston, Birkhauser Boston, 1994, 63-66.
- Long TC, Saleh N, Tilton RD, Lowry GV, Veronesi B: Titanium Dioxide (P25) Produces Reactive Oxygen Species in Immortalized Brain Microglia (BV2): Implications for Nanoparticle Neurotoxicity. Environmental Science & Technology. 2006, 40: 4346-4352. 10.1021/es060589n.
- Xia T, Kovochich M, Brant J, Hotze M, Sempf J, Oberley T, Sioutas C, Yeh JI, Wiesner MR, Nel AE: Comparison of the Abilities of Ambient and Manufactured Nanoparticles To Induce Cellular Toxicity According to an Oxidative Stress Paradigm. Nano Letters. 2006, 6: 1794-1807. 10.1021/nl061025k.
- Julian D, April KL, Patel S, Stein JR, Wohlgemuth SE: Mitochondrial depolarization following hydrogen sulfide exposure in erythrocytes from a sulfide-tolerant marine invertebrate. Journal of Experimental Biology. 2005, 208: 4109-4122. 10.1242/jeb.01867.
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.